General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.98 g/cm³ Show Material materials with Density of 7.98 g/cm³ |

Mechanical

Property | Temperature | Value | Comment |
---|---|---|---|

Elastic modulus | -100.0 °C | 206 GPa Show Material materials with Elastic modulus of 206 GPa | |

20.0 °C | 196 GPa Show Material materials with Elastic modulus of 196 GPa | ||

100.0 °C | 190 GPa Show Material materials with Elastic modulus of 190 GPa | ||

200.0 °C | 182 GPa Show Material materials with Elastic modulus of 182 GPa | ||

300.0 °C | 174 GPa Show Material materials with Elastic modulus of 174 GPa | ||

400.0 °C | 166 GPa Show Material materials with Elastic modulus of 166 GPa | ||

500.0 °C | 158 GPa Show Material materials with Elastic modulus of 158 GPa | ||

600.0 °C | 150 GPa Show Material materials with Elastic modulus of 150 GPa | ||

700.0 °C | 142 GPa Show Material materials with Elastic modulus of 142 GPa | ||

800.0 °C | 134 GPa Show Material materials with Elastic modulus of 134 GPa | ||

900.0 °C | 127 GPa Show Material materials with Elastic modulus of 127 GPa | ||

1000.0 °C | 120 GPa Show Material materials with Elastic modulus of 120 GPa | ||

Elongation | 20.0 °C | 35 % Show Material materials with Elongation of 35 % | |

Elongation, transverse | 20.0 °C | 30 % Show Material materials with Elongation, transverse of 30 % | |

Poisson's ratio | 23.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | Typical for Austenitic Stainless Steel |

Shear modulus | 23.0 °C | 77 GPa Show Material materials with Shear modulus of 77 GPa | Typical for Austenitic Stainless Steel |

Tensile strength | 20.0 °C | 490 - 690 MPa Show Material materials with Tensile strength of 490 - 690 MPa | |

Tensile strength, transverse | 20.0 °C | 490 - 690 MPa Show Material materials with Tensile strength, transverse of 490 - 690 MPa | |

Yield strength Rp0.2 | 20.0 °C | 205 MPa Show Material materials with Yield strength Rp0.2 of 205 MPa | |

100.0 °C | 177 MPa Show Material materials with Yield strength Rp0.2 of 177 MPa | ||

200.0 °C | 147 MPa Show Material materials with Yield strength Rp0.2 of 147 MPa | ||

300.0 °C | 127 MPa Show Material materials with Yield strength Rp0.2 of 127 MPa | ||

400.0 °C | 118 MPa Show Material materials with Yield strength Rp0.2 of 118 MPa | ||

500.0 °C | 108 MPa Show Material materials with Yield strength Rp0.2 of 108 MPa | ||

550.0 °C | 103 MPa Show Material materials with Yield strength Rp0.2 of 103 MPa | ||

600.0 °C | 98 MPa Show Material materials with Yield strength Rp0.2 of 98 MPa | ||

Unlock all property charts | |||

Yield strength Rp0.2, transverse | 20.0 °C | 205 MPa Show Material materials with Yield strength Rp0.2, transverse of 205 MPa | |

Yield strength Rp1.0 | 20.0 °C | 245 MPa Show Material materials with Yield strength Rp1.0 of 245 MPa | |

100.0 °C | 211 MPa Show Material materials with Yield strength Rp1.0 of 211 MPa | ||

200.0 °C | 177 MPa Show Material materials with Yield strength Rp1.0 of 177 MPa | ||

300.0 °C | 157 MPa Show Material materials with Yield strength Rp1.0 of 157 MPa | ||

400.0 °C | 147 MPa Show Material materials with Yield strength Rp1.0 of 147 MPa | ||

500.0 °C | 137 MPa Show Material materials with Yield strength Rp1.0 of 137 MPa | ||

550.0 °C | 132 MPa Show Material materials with Yield strength Rp1.0 of 132 MPa | ||

600.0 °C | 128 MPa Show Material materials with Yield strength Rp1.0 of 128 MPa | ||

Unlock all property charts | |||

Yield strength Rp1.0, transverse | 20.0 °C | 245 MPa Show Material materials with Yield strength Rp1.0, transverse of 245 MPa |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | -100.0 °C | 1.49E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.49E-5 1/K | |

20.0 °C | 1.61E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.61E-5 1/K | ||

100.0 °C | 1.67E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.67E-5 1/K | ||

200.0 °C | 1.72E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.72E-5 1/K | ||

300.0 °C | 1.77E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.77E-5 1/K | ||

400.0 °C | 1.81E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.81E-5 1/K | ||

500.0 °C | 1.84E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.84E-5 1/K | ||

600.0 °C | 1.88E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.88E-5 1/K | ||

700.0 °C | 1.91E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.91E-5 1/K | ||

800.0 °C | 1.94E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.94E-5 1/K | ||

900.0 °C | 1.97E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.97E-5 1/K | ||

1000.0 °C | 2E-5 1/K Show Material materials with Coefficient of thermal expansion of 2E-5 1/K | ||

Unlock all property charts | |||

Melting point | 1230 - 1480 °C Show Material materials with Melting point of 1230 - 1480 °C | Typical for Austenitic Stainless Steel | |

Specific heat capacity | -100.0 °C | 440 J/(kg·K) Show Material materials with Specific heat capacity of 440 J/(kg·K) | |

20.0 °C | 472 J/(kg·K) Show Material materials with Specific heat capacity of 472 J/(kg·K) | ||

100.0 °C | 487 J/(kg·K) Show Material materials with Specific heat capacity of 487 J/(kg·K) | ||

200.0 °C | 503 J/(kg·K) Show Material materials with Specific heat capacity of 503 J/(kg·K) | ||

300.0 °C | 512 J/(kg·K) Show Material materials with Specific heat capacity of 512 J/(kg·K) | ||

400.0 °C | 520 J/(kg·K) Show Material materials with Specific heat capacity of 520 J/(kg·K) | ||

500.0 °C | 530 J/(kg·K) Show Material materials with Specific heat capacity of 530 J/(kg·K) | ||

600.0 °C | 541 J/(kg·K) Show Material materials with Specific heat capacity of 541 J/(kg·K) | ||

700.0 °C | 551 J/(kg·K) Show Material materials with Specific heat capacity of 551 J/(kg·K) | ||

800.0 °C | 559 J/(kg·K) Show Material materials with Specific heat capacity of 559 J/(kg·K) | ||

900.0 °C | 565 J/(kg·K) Show Material materials with Specific heat capacity of 565 J/(kg·K) | ||

1000.0 °C | 571 J/(kg·K) Show Material materials with Specific heat capacity of 571 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 13.5 W/(m·K) Show Material materials with Thermal conductivity of 13.5 W/(m·K) | |

100.0 °C | 15 W/(m·K) Show Material materials with Thermal conductivity of 15 W/(m·K) | ||

200.0 °C | 16.7 W/(m·K) Show Material materials with Thermal conductivity of 16.7 W/(m·K) | ||

300.0 °C | 18.3 W/(m·K) Show Material materials with Thermal conductivity of 18.3 W/(m·K) | ||

400.0 °C | 19.8 W/(m·K) Show Material materials with Thermal conductivity of 19.8 W/(m·K) | ||

500.0 °C | 21.2 W/(m·K) Show Material materials with Thermal conductivity of 21.2 W/(m·K) | ||

600.0 °C | 22.7 W/(m·K) Show Material materials with Thermal conductivity of 22.7 W/(m·K) | ||

700.0 °C | 24.1 W/(m·K) Show Material materials with Thermal conductivity of 24.1 W/(m·K) | ||

800.0 °C | 25.5 W/(m·K) Show Material materials with Thermal conductivity of 25.5 W/(m·K) | ||

900.0 °C | 26.9 W/(m·K) Show Material materials with Thermal conductivity of 26.9 W/(m·K) | ||

1000.0 °C | 28.3 W/(m·K) Show Material materials with Thermal conductivity of 28.3 W/(m·K) | ||

Unlock all property charts | |||

Thermal diffusivity | 20.0 °C | 3.6 mm²/s Show Material materials with Thermal diffusivity of 3.6 mm²/s | |

100.0 °C | 3.8 mm²/s Show Material materials with Thermal diffusivity of 3.8 mm²/s | ||

200.0 °C | 4 mm²/s Show Material materials with Thermal diffusivity of 4 mm²/s | ||

300.0 °C | 4.4 mm²/s Show Material materials with Thermal diffusivity of 4.4 mm²/s | ||

400.0 °C | 4.6 mm²/s Show Material materials with Thermal diffusivity of 4.6 mm²/s | ||

500.0 °C | 4.7 mm²/s Show Material materials with Thermal diffusivity of 4.7 mm²/s | ||

600.0 °C | 4.9 mm²/s Show Material materials with Thermal diffusivity of 4.9 mm²/s | ||

700.0 °C | 5.2 mm²/s Show Material materials with Thermal diffusivity of 5.2 mm²/s | ||

800.0 °C | 5.5 mm²/s Show Material materials with Thermal diffusivity of 5.5 mm²/s | ||

900.0 °C | 5.8 mm²/s Show Material materials with Thermal diffusivity of 5.8 mm²/s | ||

1000.0 °C | 5.9 mm²/s Show Material materials with Thermal diffusivity of 5.9 mm²/s | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 7.7E-7 Ω·m Show Material materials with Electrical resistivity of 7.7E-7 Ω·m |

100.0 °C | 8.34E-7 Ω·m Show Material materials with Electrical resistivity of 8.34E-7 Ω·m | |

200.0 °C | 9.03E-7 Ω·m Show Material materials with Electrical resistivity of 9.03E-7 Ω·m | |

300.0 °C | 9.64E-7 Ω·m Show Material materials with Electrical resistivity of 9.64E-7 Ω·m | |

400.0 °C | 1.02E-6 Ω·m Show Material materials with Electrical resistivity of 1.02E-6 Ω·m | |

500.0 °C | 1.06E-6 Ω·m Show Material materials with Electrical resistivity of 1.06E-6 Ω·m | |

600.0 °C | 1.1E-6 Ω·m Show Material materials with Electrical resistivity of 1.1E-6 Ω·m | |

700.0 °C | 1.13E-6 Ω·m Show Material materials with Electrical resistivity of 1.13E-6 Ω·m | |

800.0 °C | 1.17E-6 Ω·m Show Material materials with Electrical resistivity of 1.17E-6 Ω·m | |

900.0 °C | 1.19E-6 Ω·m Show Material materials with Electrical resistivity of 1.19E-6 Ω·m | |

1000.0 °C | 1.22E-6 Ω·m Show Material materials with Electrical resistivity of 1.22E-6 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Carbon | 0.04 - 0.08 % Show Material materials with Carbon of 0.04 - 0.08 % |

Chromium | 16 - 18 % Show Material materials with Chromium of 16 - 18 % |

Manganese | 2 % Show Material materials with Manganese of 2 % |

Molybdenum | 2 - 2.5 % Show Material materials with Molybdenum of 2 - 2.5 % |

Nickel | 12 - 14 % Show Material materials with Nickel of 12 - 14 % |

Phosphorus | 0.04 % Show Material materials with Phosphorus of 0.04 % |

Silicon | 0.75 % Show Material materials with Silicon of 0.75 % |

Sulfur | 0.015 % Show Material materials with Sulfur of 0.015 % |